EPJ Web of Conferences 48, 00028 (2013) DOI: 10.1051/epjconf/20134800028 © Owned by the authors, published by EDP Sciences, 2013
J. Václavík, D. Vápenka
Institute of Plasma Physics ASCR v.v.i., TOPTEC, Sobotecká 1660, 51101 Turnov, Czech Republic
Abstract. Gallium phosphide is interesting material for optical system working in both visible and MWIR or LWIR spectral ranges. Number of a material available for these applications is limited. They are typically salts, fluorides or sulphides and usually exhibit unfavorable properties like brittleness; softness; solubility in water and small chemical resistance. Although GaP has do not offer best optical parameters excels over most other material in mechanical and chemical resistance. The article describes its most important characteristics and outlines some applications where GaP should prove useful.
1 Introduction mostly used as a semiconductor substrate for high speed electronic and optoelectronic circuits but also as lens TOPTEC research centre is working on research project material for high power infrared optics where it compete that includes production of optical elements from gallium with ZnS and ZnSe materials. Typical application of phosphide and design of infrared and combined visible- GaAs lenses is refractive optics for CO2 lasers in cutting infrared system. As the number of materials applicable in and marking machines. Although it is not best material by those systems is very limited, GaP important is one a few optical means it wins over other materials by a higher optical materials that are useable in such designs. mechanical strength, chemical resistance, thermal Gallium phosphide crystal is shown in figure 1. It is conductivity and hardness. widely used as a type III-V semiconductor material in GaP exhibits the same good mechanical properties as a LED production. Thanks to 2.26 eV wide bandgap has GaAs but differs in spectral transmission range, which is LED produced solely from GaP emission peak at 555 nm. shifted to shorter wavelengths – from 0.6 to 11 μm. Such Emitted light is designated as pure green color, but transmission range opens ways to use a GaP in visible conversion efficiency is only 0.1 % due to indirect and near infrared application where most of interesting bandgap of a pure GaP. Therefore dopants like nitrogen, infrared materials is unusable due to absorption. As a zinc or oxygen are used in order to increase LED number of materials available for building combined effifiency. Dopants allow increasing of efficiency more VIS-IR optical systems is quite limited, adding another than 100 times, but the efficiency of doped green GaP one with different properties allows more freedom in LED does not exceed 3 %. such designs. LEDs with longer central wavelength are produced from material where portion of gallium or phosphorus atoms in crystal’s lattice are replaced by different elements. Typical mixed crystal used here is InXGa(1-X)AsYP(1-Y) or AlInXGa(1-X)P . Such combinations allow good control of bandgap width over wide range, starting from 1.42 eV of GaAs to 2.26 eV of pure GaP. Some o those combined crystals also exhibits direct bandgaps. Properly selected combination is also transparent for emitted wavelength which further leads to an increased extraction efficiency. Most LEDs based on this technology have central wavelength at 565, 585, 605 and 635 nm. Especially interesting are 635 nm LEDs which have efficiency around 30 % . Gallium phosphide is not just a semiconductor substrate. It is an interesting material for optical application in the Fig. 1. 2” LEC GaP ingot produced by ITME (Instytut Technologii Materiałów Elektronicznych, Poland) same matter as gallium arsenide. Gallium arsenide is
This is an Open Access article distributed under the terms of the Creative Commons Attribution License 2.0, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Article available at http://www.epj-conferences.org or http://dx.doi.org/10.1051/epjconf/20134800028 EPJ Web of Conferences
but it is, in the same time, hampered by strong dispersion of refractive index near absorption edge of GaP as is shown in Fig 4. Therefore favorable applications lie in 800–1000 nm spectral region which is not part of VIS range but still within sensitivity of Si-based detectors. On the other hand the same dispersion and high refractive index allows design of achromatic pair in combination with ZnSe element. Production example of such lenses is displayed in figure 2. High refractive index requires high quality antireflection Fig. 2. ZnSe (left) and GaP (rigth) optical elements of coating. So far coatings containing 2 and 4 layers of bichromatic lenses for VIS and MWIR application either SiO2-TiO2 or HfO2-ZnS were realized. Antireflection coating were dual-band having minimum reflectivity at 850nm and 4µm. Those coatings were used 2 GaP properties in VIS-MWIR optics for cutting tool diagnostics.
Evaluating GaP strictly by optical properties will lead into assumption that there are much better materials actually available. Effectively useable spectral range spans from 570 nm to 11 μm which partially limits its use in visible range. There are other materials covering visible to mid infrared range much better – i.e. ZnS, CaF2 or BaF2. In the infrared end of transmission spectra the GaP losses to materials like ZnSe, BaF2 or salts like KBr. Furthermore it exhibits strong dispersion of refractive index in VIS and NIR due to absorption edge at 555 nm. Transmissivity of GaP and other materials from table 1 is show in figure 3. What makes GaP interesting is combination of its main properties  - Transparency from VIS to LWIR - High refractive index - High refractive index dispersion in VIS - Mechanical durability - Verdet constant: 160 rad.m-1.T-1 @ 633 nm Some of its important properties are summarized in table 1. Average refractive index of GaP is 3.1. It makes GaP material with highest value of refractive index for given transparency in VIS range. It lifts up some Fig. 3. Transmissivity of different VIS-IR materials in the range constrains in design of fast lenses and optical elements, 0.3-20µm. [3, 4, 8]
Table 1. Overview of material properties of various optical materials compared to GaP. [3, 4, 6-10]
GaP GaAs ZnSe ZnS Sapphire CaF2 BK7
Refractive Index 3.16 3.42 2.46 2.28 1.75 1.43 1.5 at 1.4µm
Transmissibility 0.6 – 11 0.9 - 16 0.55-19 0.45-11 0.22-4.5 0.15 – 9 0.33 – 2.3 at 50%
Thermooptical 100 250 59-70 50 10 -4 3 Coeficient at (10-6 K-1) (at 1.1µm) (at 1.1µm) (at 1.1µm) (at 1.1µm) (at 0.6µm) (at 1.1µm) (at 0.6µm) Knoop Hardness -2 850 750 105-120 160-220 1700 158 520 (kg.mm )
Flexural Strength 100 55 50 60 500-1060 90 50 (MPa) Fracture 0.4 0.33-0.5 Thoughness KIC 0.9 (orientation- (polycrystali 0,5 3 0.5 0.82 – 1.1 (MPa.m1/2) depended) ne) Price [€/kg] 4500 2200 1800 1400 3000 600 70
00028-p.2 Optics and Measurement 2012
Mechanical durability is the most important parameter of lattice dislocations and improves optical transmission of the GaP material. Materials with similar transmission the crystal. Market for optical quality GaP crystals is still range are usually brittle, soft and sensitive to thermal small and investment into development of a VGF shocks . GaP itself is harder than common optical technology quite large. Authors do not know any glasses (BK7), fracture toughness the same or higher than company with successful production using this method. of glass and its flexural strength is also significantly On the other hand there are companies producing quality higher. It is insoluble in water and has high acid and GaAs crystals by VGF method. alkali resistance. GaP is very durable material compared to commonly used VIS-IR materials like BaF2, CaF2, ZnS, ZnSe, Kbr, KCl. It is suitable as a material for 4 Production of GaP optical elements optical elements exposed to mechanical strain, harsh SPDT is most versatile method for processing infrared weather conditions or abrasive dust – i.e. windows, cover materials like ZnS, ZnSe or GaAs, but producing optical domes or front elements of optical systems. surfaces for VIS range on GaP is problematic. The TOPEC research centre produces optical elements from GaP with planar and spherical surfaces by optimized grinding-lapping-polishing cycle. Most problematic behavior of GaP is production of phosphine PH3 whenever phosphorus atoms on the surface can react with water. PH3 is very dangerous gas  and all manufacturing steps must be handled with caution and proper equipment. For a bulk material and surfaces of optical elements it is not a problem, because only a very small portion of phosphorus atoms is exposed. A large surface area is constantly opened during grinding and polishing processes and fresh phosphorus atoms are exposed. Production of PH3 becomes significant. There are two ways to inhibit production of PH3. First is eliminating water from production process – i.e. using alcohols or oils as replacement of the water in grinding and polishing slurries. Use of oils or alcohols creates serious problem with waste separation and disposal, which increases running costs. Second solution, chosen Fig. 4. Refractive indices of various VIS-IR materials as by the TOPTEC centre, is use of additives in water based a function of wavelength in range 0,6-10µm. [3,4] slurries, which causes immediate oxidation of PH3 dissolved in the slurry. By-product of this process is small amount of phosphorus acid. 3 GaP production Grinding and polishing of spherical surfaces on GaP proves to be problematic due to the anisotropy of the GaP useable for optical application must be udoped, have crystal and etching effects of additives that suppress minimum of lattice dislocation and minimum free production of PH3. It causes unequal removal rates at carriers. Free carriers causes bulk absorption of light in different angles and different positions on the surface of the material at longer wavelength. Minimal specifications produced element. for GaP optical material are: - Undoped material - Carrier concentration: <1016 cm-3 - EPD (Etch Pit Density): <5.103 cm-2 GaP crystal is grown byt LEC (Liquid Encapsulated Czochralski) method. It is well-proven method used by most semiconductor producers to grow III-V semiconductor crystals. Undoped crystals with very high quality, suitable for optical application, are not produced together with material for electronic application. The reason is necessity to fine tune growth a pull process in order to eliminate most of lattice dislocation from produced crystals. Such production is expensive for semiconductor industry. Therefore optical quality GaP is produced by companies specialized in growth of optical crystals. Another promising method is VGF (Vertical Gradient Fig. 5. MWIR objectives with GaP elements and 47mm Freeze) method which allows control over temperature aperture produced for GfE - Gesellschaft fuer Fertigungstechnik gradient in crystallization zone. This reduces amount of und Entwicklung e.V., Schmalkalden (Germany).
00028-p.3 EPJ Web of Conferences
5 Application example mechanical toughness and chemical resistivity compared to other materials in its family. Many of the possible applications of GaP material in as It was shown that high refractive index in visible range an optical element are focused on mixed VIS-IR systems. offered by this material can be useful in reducing It could be for example an optical element of thermal geometrical aberration. imager that needs common optical path for visible and Material releases dangerous substances during infrared detectors. mechanical processing and its anisotropy leads to Let’s have a simpler problem - creating single lens for irregular removal rates in polishing. TOPTEC research focusing or collimating laser beam at 1064 nm with center successfully produces spherical and planar optical smallest possible spot for given focal length. This elements from GaP and currently works on improvement example was chosen to emphasize importance of very of manufacturing process. high refractive of this material. As the application is monochromatic a low dispersion materials like CaF2 do This work was supported by the European Regional not offer any advantage. Table 2 shows parameters of Development Fund and the Ministry of Education, Youth lenses with EFL = 60mm, F/3 produced from different and Sports of the Czech Republic in the Project No. materials. Dimensions of the lens and meaning of CZ.1.05/2.1.00/03.0079: Research Center for Special parameters in the table 2 is closely explained in drawing Optics and Optoelectronic Systems (TOPTEC) and in figure 6. Shapes of these lenses were calculated in Project EUREKA E!3869 Infrasens OE10003. ZEMAX software. It clearly shows that GaP can produce more than six-times smaller focused spot than lens made References from CaF2. Example of another lenses produced from GaP is 1. F. Ye, ECE226 Optoel. Dev., (2012) displayed in figure 5. These lenses were produced as 2. M. M. El-Nahass, H. S. Metwally, H. E. A. El- objective for MWIR line-scan camera measuring Sayed, F. Abd El-salam, H. A. Hassan, Eur. Phys. J. temperature of a punching tool. App. Phys., 43, 31 (2008), High dispersion of refractive index can be exploited in 3. E. D. Palik, Handbook of Optical Constants, Vol.1, systems where a compact refractive dispersion element is (1985) required. 4. E. D. Palik, Handbook of Optical Constants, Vol.2, Table 2. Comparison of spot sizes and geometric parameters of (1991) lenses with EFL = 60 mm and f/3 at λ=1064 nm made from 5. E. D. Palik, Handbook of Optical Constants, Vol.3, various optical material (1998) 6. Marvin J. WEBER, Handbook of optical materials, GaP ZnSe ZnS Saphire CaF2 BK7 (2003) Spot 7. C. P. Chen, JPL Publication, 84-81, (1984) radii 9.5 13.7 15.9 29.7 61.3 49.3 CVD-ZnSe (um) 8. TYDEX Optics, , (2012) R 9. S. W. Freiman, JOHN J. Mecholsky Jr., ROY W. 1 58.47 54.73 52.85 44.1 33.93 36.86 (mm) Rice, J. C. Wurst, J. of the Amer. Cer. Soc., 58, 406, R (1975) 2 99.53 129.9 151.7 890.9 -129.5 -212.4 (mm) 10. W. Vidrine, Mechanical properties of transmissive optical materials, (2012) 60 11. Ch. Salocks, K. B. Kaley, PHOSPHINE (2012)
R1 20 R2
Fig. 6. Dimension of laser focusing lens shown as an example of GaP application.
GaP is a member of family of optical materials usable from VIS do 10µm spectral range. As the family does not have many members compared to VIS/NIR and MWIR/LWIR families, specific optical properties gives optical designer another free parameters to solve optical problems. Important characteristic of GaP is its